[BS 1016-104.3-1998] -- Methods for analysis and testing of coal and coke..pdf
Download [BS 1016-104.3-1998] -- Methods for analysis and testing of coal and coke..pdf...
Methods for analysis and testing of coal and coke — Part 104: Proximate analysis — Section 104.3: Determination of volatile matter content
ICS 73,0 73,040; 40; 75.1 75.160.1 60.10 0
BS 10 1016 16-1 -104 04.3: .3: 1998 ISO 56 562:1 2:199 998 8
National foreword This British Standard is the UK implementation of ISO 562:1998. It supersedes BS 1016-104.3:1991 which is withdrawn. The UK participation in its preparation was entrusted to Technical Committee SFI/3, Analysis and testing of coal and coke, which has the responsibility to: — aid enquirers to understand the text; — present to the responsible international/European committee any enquiries on the interpretation, or proposals for change, and keep the UK interests informed; — monitor related international and European developments and promulgate them in the UK. A list of organizations represented on this committee can be obtained on request to its secretary. Cross-references
The British Standards which implement international or European publications referred to in this document may be found in the BSI Standards Catalogue under the section entitled “International Standards Correspondence Index”, or by using the “Find” facility of the BSI Standards Electronic Catalogue. A British Standard does not purport to include all the necessary provisions of a contract. Users of British Standards are responsible for their correct application. Compliance with a British Standard does not of itself confer immunity from legal obligations.
Summary of pages
This document comprises a front cover, an inside front cover, pages i and ii, the ISO title page, page ii, pages 1 to 6 and a back cover. This standard has been updated (see copyright date) and may have ha d amendments incorporated. This will be indicated in the amendment table on the inside front cover.
This British Standard, having been prepared under the direction of the Sector Board for Materials and Chemicals, was published under the authority of the Standards Board and comes into effect on 15 April 1998 © BSI 04-1999
ISBN 0 580 29677 6
Amendments issued since publication
National foreword Foreword Introduction 1 Scope 2 Normative references 3 Principle 4 Reagent 5 Apparatus 6 Preparation of the test sample 7 Procedure 8 Expression of results 9 Precision 10 Test report Annex A (informative) Bibliography Figure 1 — Example of suitable furnace Figure 2 — Silica crucible and lid Figure 3 — Crucible stands Table 1
© BSI 04-1999
Page Inside front cover iii 1 1 1 1 1 1 4 4 5 5 5 6 2 3 4 5
BS 1016-104.3:1998 Foreword ISO (the International Organization for Standardization) is a worldwide federation of national standards bodies (ISO member bodies). The work of preparing International Standards is normally carried out through ISO technical committees. Each member body interested in a subject for which a technical committee has been established has the right to be represented on that committee. International organizations, governmental and non-governmental, in liaison with ISO, also take part in the work. ISO collaborates closely with the International Electrotechnical Commission (IEC) on all matters of electrotechnical standardization. Draft International Standards adopted by the technical committees are circulated to the member bodies for voting. Publication as an International Standard requires approval by at least 75 % of the member bodies casting a vote. International Standard ISO 562 was prepared by Technical Committee ISO/TC 27, Solid mineral fuels, Subcommittee SC 5, Methods of analysis. This second edition cancels and replaces the first edition (ISO 562:1981), which has been technically revised. Annex A of this International Standard is for information only.
Descriptors: Solid fuels, fossil fuels, coal, pit-coal, coke, tests, determination of content, volatile matter, gravimetric analysis, test equipment.
© BSI 04-1999
The volatile matter is determined as the loss in mass, less that due to moisture, when coal or coke is heated out of contact with air under standardized conditions. The test is empirical and, in order to ensure reproducible results, it is essential that the rate of heating, the final temperature and the overall duration of the test are carefully controlled. It is also essential to exclude air from the coal or coke during heating to prevent oxidation. The fit of the crucible lid is therefore critical. The moisture content of the sample is determined at the same time as the volatile matter so that the appropriate correction can be made.
A portion of the sample is heated out of contact with air at 900 °C for 7 min. The percentage of volatile matter is calculated from the loss in mass of the test portion after deducting the loss in mass due to moisture.
Mineral matter associated with the sample may also lose mass under the conditions of the test, the magnitude of the loss being dependent on both the nature and the quantity of the minerals present. NOTE When applying this International Standard for classification purposes, to samples obtained directly from coal seams, special care has to be given to the ash content.
The apparatus and procedure are specified so that one or more determinations may be performed simultaneously in the furnace.
1 Scope This International Standard specifies a method of determining the volatile matter of hard coal and of coke. It is not applicable to brown coals and lignites.
2 Normative references
4 Reagent Cyclohexane of recognized analytical grade.
5 Apparatus 5.1 Furnace, heated by electricity, in which a zone of uniform temperature of 900 °C ± 5 °C can be maintained. It may be of the stop-ended type or fitted at the back with a flue approximately 25 mm diameter and 150 mm long (see Figure 1). NOTE It is important for furnaces with flues that the furnace door seal well. The flue should not reach far out of the oven and should be fitted with a butterfly valve to restrict airflow through the furnace.
Its heat capacity shall be such that, with an initial temperature of 900 °C, the temperature is regained within 4 min after insertion of a cold stand and its crucibles. The temperature is measured with a thermocouple, as described in 5.2. Normally the furnace will be designed specifically either for multiple determinations using a number of crucibles in one stand or for receiving one crucible and its stand. In the first case, the zone of uniform temperature shall be at least 160 mm × 100 mm; in the latter case, a zone of diameter 40 mm will be sufficient.
The following standards contain provisions which, through reference in this text, constitute provisions A position for the crucible stand shall be chosen within the zone of uniform temperature and this of this International Standard. At the time of position shall be used for all determinations. The publication, the editions indicated were valid. All temperature of 900 °C shall be attained as closely as standards are subject to revision, and parties to possible with a specified tolerance of ± 5 °C in order agreements based on this International Standard to compensate for inherent errors in the are encouraged to investigate the possibility of temperature measurement and lack of uniformity in applying the most recent editions of the standards indicated below. Members of IEC and ISO maintain the temperature distribution. registers of currently valid International Standards. 5.2 Thermocouple, unsheathed, of wire no thicker ISO 331:1983, Coal — Determination of moisture in than 1 mm. It should be long enough to reach the centre of the underside of each crucible when placed the analysis sample — Direct gravimetric method. in the zone of uniform temperature on being ISO 687:1974, Coke — Determination of moisture in inserted through the front or rear of the furnace. the analysis sample. The thermojunction shall be placed midway ISO 11722:— 1), Solid mineral fuels — Hard coal — between the base of the crucible in its stand and the Determination of moisture in the analysis sample by floor of the furnace. If the stand holds more than one drying in nitrogen. crucible, the temperature under each crucible shall be checked in the same manner.
© BSI 04-1999
If desired, a sheathed thermocouple may be permanently installed in the furnace (see Figure 1) with its thermojunction as close as possible to the centre of the zone of uniform temperature; in this case furnace temperature readings shall be correlated at frequent intervals with those of the unsheathed thermocouple, which is thus inserted only when necessary. NOTE The temperature/electromotive force relationship of a thermojunction maintained at elevated temperatures gradually changes with time.
5.3 Crucible, cylindrical, with a well-fitting lid, both of fused silica. The crucible with lid shall have a mass between 10 g and 14 g and dimensions approximating to those shown in Figure 2. The fit of the lid on the crucible is critical to the determination and a lid shall be selected to match the crucible so that the horizontal clearance between them is no greater than 0,5 mm. After selection, the crucible and the lid shall be ground together to give smooth surfaces and then be given a common distinguishing mark.
NOTE When performing multiple determinations on highly swelling coals, it may be necessary to use taller crucibles; these may be up to 45 mm in height without affecting the determined volatile matter, provided that the specified rate of temperature recovery be maintained.
5.4 Crucible stand, on which the crucible is placed in the furnace, such that the appropriate rate of heating can be achieved. For example, it may consist of the following:
a) for single determinations, a ring of heat-resistant steel wire as shown in Figure 3 a) with ceramic discs, 25 mm diameter and 2 mm thick, resting on the inner projection of its legs or b) for multiple determinations, a tray of heat-resistant steel wire as shown in Figure 3 b), of appropriate size, with ceramic plates 2 mm thick supporting the crucibles. 5.5 Balance, capable of reading to the nearest 0,1 mg.
Figure 1 — Example of suitable furnace
© BSI 04-1999
Figure 2 — Silica crucible and lid
© BSI 04-1999
Figure 3 — Crucible stands
6 Preparation of the test sample
The coal or coke used for the determination of volatile matter is the general analysis test sample (ground to pass a sieve of 212 µm aperture). The sample shall be well mixed and in moisture equilibrium with the laboratory atmosphere.
7.1 Furnace temperature checking
A test portion from the same test sample is separated for determination of moisture parallel to the determination of volatile matter.
Adjust the temperature of the zone in the furnace (5.1), containing either a stand with one crucible and lid [Figure 3 a)] or a stand with the requisite number of crucibles and lids [Figure 3 b)], to 900 °C ± 5 °C as indicated by the correctly located thermocouple (5.2). Check that the temperature under each crucible, at the same height, lies within the temperature tolerance of the uniform zone.
© BSI 04-1999
NOTE Temperature checking should be made before starting determinations. However, when several analyses are performed per day, a daily temperature check is sufficient. The check of the temperature recovery criterion (5.1) should be dealt with in a similar way.
7.2 Volatile matter determination
Fill either a stand with one empty crucible and lid [Figure 3 a)] or a stand with the requisite number of empty crucibles and lids [Figure 3 b)] and insert in the oven. Maintain at 900 °C ± 5 °C for 7 min. Remove the crucible(s) from the furnace and allow to cool to room temperature on a thick metal plate. As soon as they are cool, weigh each empty crucible and lid and weigh into each crucible, to the nearest 0,1 mg, 1 ± 0,1 g of test sample. Replace the lid and tap each crucible on a clean hard surface until the test portion forms a layer of even thickness on the bottom of the crucible. If the sample is of coke, remove the lid of the charged crucible, add 2 to 4 drops of cyclohexane (4) and replace the lid. NOTE The addition of cyclohexane prevents oxidation of the coke but does not prevent adsorption of gases, e.g. nitrogen.
Place the charged crucible(s) in a cold stand, transfer to the furnace, close the door and leave for 7 min ± 5 s. Remove and allow to cool to room temperature. When cool, weigh the crucible(s) to the nearest 0,1 mg in the same manner as for the empty crucible(s). NOTE 1 The same treatment of the crucible before and after the determination minimizes the effect of any film of water adsorbed on its surface, while the rapid cooling reduces absorption of moisture by the coal or coke residue. NOTE 2 If multiple determinations are being made, any vacant places in the stand should be filled with empty crucibles.
8 Expression of results The volatile matter V in the sample as analysed, expressed as a percentage by mass, is given by the equation: 100 ( m 2 – m 3 ) V = ------------------------------------- – M ( m 2 – m 1 )
Report the result, as the mean of duplicate determinations, to the nearest 0,1 % (m/m). The results of the determination described in this International Standard are reported on the “air-dried” basis. Calculation of the results to other bases is dealt with in ISO 1170.
9 Precision Table 1
Maximum acceptable differences between, results obtained (calculated to the same moisture content) Repeatability limit
Reproducibility critical difference
Hard coal of volatile matter < 10 %
0,3 % absolute 0,5 % absolute
Hard coal of volatile matter >10 %
3 % of the mean result
0,2 % absolute 0,3 % absolute
0,5 % absolute or 4 % of the mean result, whichever is greater
9.1 Repeatability limit
The results of the duplicate determinations (performed within a short period of time, but not simultaneously) in the same laboratory by the same operator using the same apparatus on two representative test portions taken from the same general analysis test sample, shall not differ by more than the values given in Table 1. 9.2 Reproducibility critical difference
The means of the results of duplicate determinations, performed in each of two different laboratories on representative test portions taken from the same general analysis test sample shall not differ by more than the above values.
10 Test report
The test report shall include the following information:
is the mass, in grams, of the empty crucible and lid;
is the mass, in grams, of the crucible and lid and test portion before heating;
a) the identification of the sample tested;
is the mass, in grams, of the crucible and lid and contents after heating;
c) the date of the determination;
is the moisture, as a percentage by mass, in the sample as analysed, determined according to the method specified in ISO 331 (to be superseded by ISO 11722) or ISO 687.
b) the method used; d) results of the determination performed, together with the relevant analysis basis (e.g. air dry); e) any unusual features noted during the determination; f) a reference to this International Standard; g) any operation not included in this International Standard or regarded as optional.
© BSI 04-1999
Annex A (informative) Bibliography  ISO 1170:1977, Coal and coke — Calculation of analyses to different bases.  ISO 1213-2:1992, Solid mineral fuels — Vocabulary — Part 2: Terms relating to sampling testing and analysis.
© BSI 04-1999
BS 1016-104.3: 1998 ISO 562:1998
BSI — British Standards Institution BSI is the independent national body responsible for preparing British Standards. It presents the UK view on standards in Europe and at the international level. It is incorporated by Royal Charter. Revisions
British Standards are updated by amendment or revision. Users of British Standards should make sure that they possess the latest amendments or editions. It is the constant aim of BSI to improve the quality of our products and services. We would be grateful if anyone finding an inaccuracy or ambiguity while using this British Standard would inform the Secretary of the technical committee responsible, the identity of which can be found on the inside front cover. Tel: 020 8996 9000. Fax: 020 8996 7400. BSI offers members an individual updating service called PLUS which ensures that subscribers automatically receive the latest editions of standards. Buying standards
Orders for all BSI, international and foreign standards publications should be addressed to Customer Services. Tel: 020 8996 9001. Fax: 020 8996 7001. In response to orders for international standards, it is BSI policy to supply the BSI implementation of those that have been published as British Standards, unless otherwise requested. Information on standards
BSI provides a wide range of information on national, European and international standards through its Library and its Technical Help to Exporters Service. Various BSI electronic information services are also available which give details on all its products and services. Contact the Information Centre. Tel: 020 8996 7111. Fax: 020 8996 7048. Subscribing members of BSI are kept up to date with standards developments and receive substantial discounts on the purchase price of standards. For details of these and other benefits contact Membership Administration. Tel: 020 8996 7002. Fax: 020 8996 7001. Copyright
Copyright subsists in all BSI publications. BSI also holds the copyright, in the UK, of the publications of the internationalstandardization bodies. Except as permitted under the Copyright, Designs and Patents Act 1988 no extract may be reproduced, stored in a retrieval system or transmitted in any form or by any means – electronic, photocopying, recording or otherwise – without prior written permission from BSI. This does not preclude the free use, in the course of implementing the standard, of necessary details such as symbols, and size, type or grade designations. If these details are to be used for any other purpose than implementation then the prior written permission of BSI must be obtained.
BSI 389 Chiswick High Road London W4 4AL
If permission is granted, the terms may include royalty payments or a licensing agreement. Details and advice can be obtained from the Copyright Manager. Tel: 020 8996 7070.